Output from "TOTOPOL", (version 1.92, 17 Jul 2017, Mike Treacy).

Report for the framework in file "public/tmp/tmp_194_6_100827531_YwJAFb.cif"

There are 144 T-atoms per unit cell
There are 288 O-atoms per unit cell

Framework density = 23.09 T-atoms per nm^3
Material density = 2.304 grams per cm^3 (excluding extra-framework material)
-------------------------------------------------------------------
-------------------------- T-O Analysis ---------------------------
-------------------------------------------------------------------
[Si] Ideal SiO distance = 1.610 Angstrom
T1  -- O1  = 1.6393 Angstrom
T1  -- O2  = 1.6451 Angstrom
T1  -- O3  = 1.6568 Angstrom
T1  -- O4  = 1.6748 Angstrom
      mean = 1.6540 Angstrom
        t1 = 0.045364  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.042604  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T2  -- O3  = 1.6885 Angstrom
T2  -- O5  = 1.6515 Angstrom
T2  -- O6  = 1.7416 Angstrom
T2  -- O7  = 1.6630 Angstrom
      mean = 1.6862 Angstrom
        t1 = 0.052136  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.023007  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T3  -- O4  = 1.6684 Angstrom
T3  -- O8  = 1.6496 Angstrom
T3  -- O9  = 1.6169 Angstrom
T3  -- O10 = 1.6603 Angstrom
      mean = 1.6488 Angstrom
        t1 = 0.035317  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.021019  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T4  -- O6  = 1.7077 Angstrom
T4  -- O11 = 1.5961 Angstrom
T4  -- O12 = 1.6976 Angstrom
T4  -- O13 = 1.4871 Angstrom
      mean = 1.6221 Angstrom
        t1 = 0.087344  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.120078  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T5  -- O13 = 1.5822 Angstrom
T5  -- O15 = 1.6053 Angstrom
T5  -- O7  = 1.6820 Angstrom
T5  -- O14 = 1.5763 Angstrom
      mean = 1.6114 Angstrom
        t1 = 0.069752  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.059868  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T6  -- O15 = 1.5593 Angstrom
T6  -- O16 = 1.5749 Angstrom
T6  -- O17 = 1.6088 Angstrom
T6  -- O18 = 1.5897 Angstrom
      mean = 1.5832 Angstrom
        t1 = 0.022719  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.013673  (0.0 is a perfect tetrahedron)

        T-O SUMMARY
          Range  = 1.4871 A <--> 1.7416 A
          Mean   = 1.6343 A
          StdDev = 0.0555 A

       t1 Range  = 0.0227 <-- 0.0521 --> 0.0873
       t2 Range  = 0.0137 <-- 0.0467 --> 0.1201

-------------------------------------------------------------------
------------------------- O-T-O Analysis --------------------------
-------------------------------------------------------------------
O1  -- T1  -- O2  = 105.674 deg; O1  -- O2  = 3 A
O1  -- T1  -- O3  = 101.070 deg; O1  -- O3  = 3 A
O1  -- T1  -- O4  = 117.632 deg; O1  -- O4  = 3 A
O2  -- T1  -- O3  = 113.630 deg; O2  -- O3  = 3 A
O2  -- T1  -- O4  = 107.415 deg; O2  -- O4  = 3 A
O3  -- T1  -- O4  = 111.438 deg; O3  -- O4  = 3 A
       101.070 deg <-- 109.477 deg --> 117.632 deg

O3  -- T2  -- O5  = 107.145 deg; O3  -- O5  = 3 A
O3  -- T2  -- O6  = 111.452 deg; O3  -- O6  = 3 A
O3  -- T2  -- O7  = 107.390 deg; O3  -- O7  = 3 A
O5  -- T2  -- O6  = 108.127 deg; O5  -- O6  = 3 A
O5  -- T2  -- O7  = 110.317 deg; O5  -- O7  = 3 A
O6  -- T2  -- O7  = 112.297 deg; O6  -- O7  = 3 A
       107.145 deg <-- 109.455 deg --> 112.297 deg

O4  -- T3  -- O8  = 111.895 deg; O4  -- O8  = 3 A
O4  -- T3  -- O9  = 106.615 deg; O4  -- O9  = 3 A
O4  -- T3  -- O10 = 114.976 deg; O4  -- O10 = 3 A
O8  -- T3  -- O9  = 106.635 deg; O8  -- O9  = 3 A
O8  -- T3  -- O10 = 109.547 deg; O8  -- O10 = 3 A
O9  -- T3  -- O10 = 106.661 deg; O9  -- O10 = 3 A
       106.615 deg <-- 109.388 deg --> 114.976 deg

O6  -- T4  -- O11 = 108.479 deg; O6  -- O11 = 3 A
O6  -- T4  -- O12 = 129.526 deg; O6  -- O12 = 3 A
O6  -- T4  -- O13 =  95.071 deg; O6  -- O13 = 2 A
O11 -- T4  -- O12 = 109.625 deg; O11 -- O12 = 3 A
O11 -- T4  -- O13 = 109.300 deg; O11 -- O13 = 3 A
O12 -- T4  -- O13 = 102.217 deg; O12 -- O13 = 2 A
       95.071 deg <-- 109.036 deg --> 129.526 deg

O13 -- T5  -- O15 =  94.687 deg; O13 -- O15 = 2 A
O13 -- T5  -- O7  = 117.360 deg; O13 -- O7  = 3 A
O13 -- T5  -- O14 = 108.391 deg; O13 -- O14 = 3 A
O15 -- T5  -- O7  = 124.823 deg; O15 -- O7  = 3 A
O15 -- T5  -- O14 = 107.671 deg; O15 -- O14 = 3 A
O7  -- T5  -- O14 = 103.114 deg; O7  -- O14 = 3 A
       94.687 deg <-- 109.341 deg --> 124.823 deg

O15 -- T6  -- O16 = 106.446 deg; O15 -- O16 = 3 A
O15 -- T6  -- O17 = 111.816 deg; O15 -- O17 = 3 A
O15 -- T6  -- O18 = 110.314 deg; O15 -- O18 = 3 A
O16 -- T6  -- O17 = 109.716 deg; O16 -- O17 = 3 A
O16 -- T6  -- O18 = 108.056 deg; O16 -- O18 = 3 A
O17 -- T6  -- O18 = 110.350 deg; O17 -- O18 = 3 A
       106.446 deg <-- 109.450 deg --> 111.816 deg

        O-T-O SUMMARY
          Range  = 94.6872 deg <--> 129.5257 deg
          Mean   = 109.4921 deg
          StdDev = 6.8225 deg

        O--O SUMMARY
          Range  = 2.3442 A <--> 3.0802 A
          Mean   = 2.6681 A
          StdDev = 0.1515 A

-------------------------------------------------------------------
------------------------- T-T-T Analysis --------------------------
-------------------------------------------------------------------
-------------------------------------------------------------------
------------------------- T-O-T Analysis --------------------------
-------------------------------------------------------------------
T1  -- O1  -- T1  = 173.233 deg ; T1  -- T1   3.2729 A

T1  -- O2  -- T1  = 119.688 deg ; T1  -- T1   2.8449 A

T1  -- O3  -- T2  = 134.943 deg ; T1  -- T2   3.0901 A

T1  -- O4  -- T3  = 163.332 deg ; T1  -- T3   3.3079 A

T2  -- O5  -- T2  = 148.773 deg ; T2  -- T2   3.1811 A

T2  -- O6  -- T4  = 126.884 deg ; T2  -- T4   3.0854 A

T2  -- O7  -- T5  = 167.282 deg ; T2  -- T5   3.3245 A

T3  -- O8  -- T3  = 153.906 deg ; T3  -- T3   3.2141 A

T3  -- O9  -- T3  = 128.988 deg ; T3  -- T3   2.9186 A

T3  -- O10 -- T3  = 147.923 deg ; T3  -- T3   3.1914 A

T4  -- O11 -- T4  = 134.581 deg ; T4  -- T4   2.9447 A

T4  -- O12 -- T4  = 111.477 deg ; T4  -- T4   2.8060 A

T4  -- O13 -- T5  = 114.959 deg ; T4  -- T5   2.5885 A

T5  -- O14 -- T5  = 131.325 deg ; T5  -- T5   2.8724 A

T5  -- O15 -- T6  = 148.967 deg ; T5  -- T6   3.0492 A

T6  -- O16 -- T6  = 165.776 deg ; T6  -- T6   3.1256 A

T6  -- O17 -- T6  = 123.333 deg ; T6  -- T6   2.8320 A

T6  -- O18 -- T6  = 141.504 deg ; T6  -- T6   3.0016 A


        T-O-T SUMMARY
          Range  = 111.4765° <--> 173.2328 deg
          Mean   = 140.9374 deg
          StdDev = 18.2968 deg

        T--T SUMMARY
          Range  = 2.5885 A <--> 3.3245 A
          Mean   = 3.0362 A
          StdDev = 0.1953 A

-------------------------------------------------------------------
------------------------ *** WARNINGS *** -------------------------
-------------------------------------------------------------------

T-T-T analysis was not conducted.

SOME T-ATOM DISTANCES ARE OUTSIDE THE NORMAL RANGE
T2  has 6 neighboring T-atoms within 3.50 A, but only 4 bridging O-atoms
  T2  -- T1  = 3.0901 Angstrom
  T2  -- T2  = 3.1811 Angstrom
  T2  -- T4  = 3.0854 Angstrom
  T2  -- T5  = 3.2355 Angstrom
  T2  -- T2  = 3.4981 Angstrom
  T2  -- T5  = 3.3245 Angstrom
T3  has 5 neighboring T-atoms within 3.50 A, but only 4 bridging O-atoms
  T3  -- T3  = 3.2141 Angstrom
  T3  -- T3  = 2.9186 Angstrom
  T3  -- T3  = 3.1914 Angstrom
  T3  -- T4  = 3.3617 Angstrom
  T3  -- T1  = 3.3079 Angstrom
T4  has 5 neighboring T-atoms within 3.50 A, but only 4 bridging O-atoms
  T4  -- T2  = 3.0854 Angstrom
  T4  -- T3  = 3.3617 Angstrom
  T4  -- T4  = 2.9447 Angstrom
  T4  -- T4  = 2.8060 Angstrom
  T4  -- T5  = 2.5885 Angstrom
T5  has 6 neighboring T-atoms within 3.50 A, but only 4 bridging O-atoms
  T5  -- T2  = 3.2355 Angstrom
  T5  -- T4  = 2.5885 Angstrom
  T5  -- T5  = 2.8724 Angstrom
  T5  -- T6  = 3.0492 Angstrom
  T5  -- T2  = 3.3245 Angstrom
  T5  -- T5  = 3.0261 Angstrom
T6  has 5 neighboring T-atoms within 3.50 A, but only 4 bridging O-atoms
  T6  -- T5  = 3.0492 Angstrom
  T6  -- T6  = 3.1256 Angstrom
  T6  -- T6  = 2.8320 Angstrom
  T6  -- T6  = 3.0016 Angstrom
  T6  -- T6  = 3.4207 Angstrom

-------------------------------------------------------------------
---------------------- Topological Analysis -----------------------
-------------------------------------------------------------------
T1 (Si): multiplicity = 24
Coordination Sequence =
    1 4 10 22 41 65 96 137 182 223 263 315 387 471 555 637 723
TD10 = 1044
Circuit symbol = 4.6_{2}.4.8.6.8_{3}
Weight = 21
Vertex symbol  = 4.6_{2}.4.8.8.8
Weight = 25

T2 (Si): multiplicity = 24
Coordination Sequence =
    1 4 11 24 41 61 85 117 163 221 278 327 379 447 538 644 746
TD10 = 1006
Circuit symbol = 4.6.6.8_{2}.6.8_{3}
Weight = 23
Vertex symbol  = 4.6.6.8.6.8_{2}
Weight = 23

T3 (Si): multiplicity = 24
Coordination Sequence =
    1 4 9 18 36 67 108 148 180 213 262 330 406 478 546 620 709
TD10 = 1046
Circuit symbol = 4.4.4.8_{3}.6.6_{2}
Weight = 16
Vertex symbol  = 4.4.4.8.6.8
Weight = 21

T4 (Si): multiplicity = 24
Coordination Sequence =
    1 4 9 18 35 59 84 110 144 193 259 334 404 460 508 571 665
TD10 = 916
Circuit symbol = 4.4.4.6_{2}.6.6_{2}
Weight = 16
Vertex symbol  = 4.4.4.6_{2}.6.8
Weight = 20

T5 (Si): multiplicity = 24
Coordination Sequence =
    1 4 10 20 35 56 83 118 159 205 263 332 402 467 535 616 704
TD10 = 954
Circuit symbol = 4.6_{2}.4.8.6_{2}.8_{4}
Weight = 27
Vertex symbol  = 4.6_{2}.4.8.6.8_{2}
Weight = 27

T6 (Si): multiplicity = 24
Coordination Sequence =
    1 4 9 17 31 55 89 127 166 212 273 350 435 513 569 605 650
TD10 = 984
Circuit symbol = 4.4.4.8_{4}.6_{2}.6_{2}
Weight = 19
Vertex symbol  = 4.4.4.8.6.6
Weight = 19

<TD10> = 991.667
Average ring size = 5.4972
